It is normally appropriate to send a draft copy of the minutes to all the members in advance of the meeting so that the meeting is not delayed by a reading of the draft. See also
Diary
Gazette

References
Citations
Sources
Further reading
American Institute of Parliamentarians (2014). The Complete Minutes Manual. American Institute of Parliamentarians. Archived from the original on 2016-10-14. Retrieved 2016-03-01. National Association of Parliamentarians (2009). Pathways to Proficiency - What Was Done at the Meeting: A Guide to Minutes. Independence, MO: National Association of Parliamentarians. ISBN 9781884048562. Mina, Eli (2004). Minas Guide to Minute Taking. Vancouver (Canada): Eli Mina Consulting. ISBN 978-0973442809.
W
        =
        
          
            1
            2
          
        
        c
        
          (
          
            
              e
              
                
                  b
                  
                    i
                    j
                    k
                    l
                  
                
                
                  E
                  
                    i
                    j
                  
                
                
                  E
                  
                    k
                    l
                  
                
              
            
            −
            1
          
          )
        
      
    
    {\displaystyle W={\frac {1}{2}}c\left(e^{b_{ijkl}E_{ij}E_{kl}}-1\right)}

Gent-elastic material
W
        =
        −
        
          
            
              μ
              
                J
                
                  m
                
              
            
            2
          
        
        ln
        ⁡
        
          (
          
            1
            −
            
              (
              
                
                  
                    
                      λ
                      
                        1
                      
                      
                        2
                      
                    
                    +
                    
                      λ
                      
                        2
                      
                      
                        2
                      
                    
                    +
                    
                      λ
                      
                        3
                      
                      
                        2
                      
                    
                    −
                    3
                  
                  
                    J
                    
                      m
                    
                  
                
              
              )
            
          
          )
        
      
    
    {\displaystyle W=-{\frac {\mu J_{m}}{2}}\ln \left(1-\left({\frac {\lambda _{1}^{2}+\lambda _{2}^{2}+\lambda _{3}^{2}-3}{J_{m}}}\right)\right)}
  where 
  
    
      
        μ
        >
        0
      
    
    {\displaystyle \mu >0}
   is the shear modulus for infinitesimal strains and 
  
    
      
        
          J
          
            m
          
        
        >
        0
      
    
    {\displaystyle J_{m}>0}
   is a stiffening parameter, associated with limiting chain extensibility.